- Research
- Open Access
- Published:

# An optimization method for parameter extraction of metals using modified Debye model

*SpringerPlus*
**volumeÂ 2**, ArticleÂ number:Â 426 (2013)

## Abstract

The Modified Debye Model (MDM) parameters for five metals are presented. A nonlinear optimization algorithm has been developed in order to extract the parameters for the metals. The extracted parameters have been used to determine the complex relative permittivity of the metals in optical and near-IR region of electromagnetic spectrum. The obtained results have been compared with the experimental values and an excellent agreement has been found.

## Introduction

The finite-difference time-domain (FDTD) method, proposed by Yee (1966), is one of the widely used algorithms in computational electromagnetics. The time dependent form of Maxwellâ€™s equations can be successfully integrated in this method. The major advantage of the time-domain method is that the solutions can cover a wide frequency range with a single simulation run. This reduces the computation time and memory requirement significantly.

Original formulations of Yee described the isotropic materials with static permittivity only. However, in order to simulate real dispersive materials using FDTD method, we need to incorporate the formulations of frequency dependent properties of materials in the simulation model.

Choice of ohmic contacts dramatically influences the performance of optoelectronic devices. Metallic mirrors serve as ohmic contacts as well as reflectivity enhancer in lasers and LEDs (Baba et al. 1996; Chang-Hasnain et al. 1991; Hunt et al. 1993; Katz 1995; Luo and Zory 1990; Smith et al. 1995). It has been observed that wetting metals like Palladium and Titanium provide reliable adhesion and better ohmic contacts (Yang et al. 1990). The shortcomings of noble metals like gold can be overcome by employing a thin layer of Titanium on the surface. Besides, metals are indispensable for producing surface plasmon polariton (SPP). Thin Nickel films have drawn a lot of attention of the researchers for producing long-range SPP (Zervas 1990; Yates et al. 2006; Hickernell and Sarid 1987). Therefore, modeling parameters of these metals should be available in order to simulate and investigate new techniques for optoelectronic devices. Oftentimes researchers consider perfect electric conductors in their simulation model due to the lack of appropriate modeling parameters of metals (Shi and Hesselink 2004; Shi et al. 2002).

The parameters of several metals have been reported to our knowledge. Jin *et al.* have determined the MDM (Kunz and Luebbers 1993) parameters for gold which are applicable in the wavelength range of 550â€“950Â nm (Jin and Xu 2006). Krug *et al.* have reported the gold parameters that are applicable in the wavelength range of 700-1000Â nm (Krug et al. 2002). W.H.P. Pernice *et al.* (Pernice et al. 2007) have extracted the parameters for Nickel using Lorentz-Drude model. A.D. Rakic *et al.* (Rakic et al. 1998) have reported the parameters for Nickel, Palladium, Titanium and 8 other metals using Lorentz-Drude and Brendel-Bormann Model. M.A. Ordal *et al.* (Ordal et al. 1985) have extracted the parameters for fourteen metals in the infrared and far-infrared range. However, extraction of parameters using modified Debye model (MDM) (Kunz and Luebbers 1993) for these metals have not been reported to our knowledge.

Herein, we focus on real metals which exhibit dispersive properties at high frequency. In order to integrate the frequency dependent dispersive properties of materials in the FDTD algorithm, the constitutive parameters should be denoted as constants. We use the modified Debye model (MDM) (Kunz and Luebbers 1993) to describe the frequency dependent dispersive behavior of the real metals. However, the parameters need to be extracted in order to include them in the FDTD formulations. We develop a nonlinear algorithm to extract the parameters for Nickel, Hexagonal Cobalt, Palladium, Iridium and Titanium. The obtained parameters have been used to determine the complex relative permittivity of the metals which have been compared with the experimental values (Palik 1998). From our comparison we find that the RMS deviations for the extracted parameters are as little as 1.0270, 1.1519, 0.2489, 1.6216 and 1.1239 respectively. The advantage of our extracted parameters is that it requires less computation time and exhibits less RMS deviations from the parameters reported by other researchers.

## Material model and optimization method

### Material model

The complex relative permittivity function of the modified Debye model (Kunz and Luebbers 1993) is described by the following equation,

where, *Ïµ*
_{
âˆž
} is the infinite frequency relative permittivity, *Ïµ*
_{
s
} is the zero frequency relative permittivity, *Ï‰* is the angular frequency, *Ï„* is the relaxation time and *Ïƒ* is the conductivity.

If the model is represented in terms of its real and imaginary parts, then,

where, the real part of the complex relative permittivity is, {\mathrm{\xcf\mu}}^{"}\left(\mathrm{\xcf\u2030}\right)={\mathrm{\xcf\mu}}_{\mathrm{\xe2\u02c6\u017e}}+\frac{{\mathrm{\xcf\mu}}_{s}\xe2\u02c6\u2019{\mathrm{\xcf\mu}}_{\mathrm{\xe2\u02c6\u017e}}}{\left(1+{\mathrm{\xcf\u2030}}^{2}{\mathrm{\xcf\u201e}}^{2}\right)} and the imaginary part of the complex relative permittivity is, {\mathrm{\xcf\mu}}^{"}\left(\mathrm{\xcf\u2030}\right)=\frac{\left({\mathrm{\xcf\mu}}_{s}\xe2\u02c6\u2019{\mathrm{\xcf\mu}}_{\mathrm{\xe2\u02c6\u017e}}\right)\mathit{\xcf\u2030\xcf\u201e}}{\left(1+{\mathrm{\xcf\u2030}}^{2}{\mathrm{\xcf\u201e}}^{2}\right)}+\frac{\mathrm{\xcf\u0192}}{\mathrm{\xcf\u2030}{\mathrm{\xcf\mu}}_{o}}.

From (1), we can see that the modified Debye model can be described by four parameters which are *Ïµ*
_{
âˆž
}, *Ïµ*
_{
s
}, *Ï„* and *Ïƒ*. However, a relationship can be derived among these parameters by comparing (1) with the Drude model equation as,

Now we actually have three parameters that need to be extracted and the other can be obtained from (3).

### Optimization method

The equation describing the modified Debye model is nonlinear in nature which is why it is difficult to develop an optimization algorithm that can perfectly extract the modeling parameters. However, we have developed a minimization algorithm that utilizes the least-squares technique.

The algorithm that we have used is as follows. First we obtain the experimental values from the book of Palik (Palik 1998) and use them to obtain the complex relative permittivity for each material. Then the program varies the three parameters that need to be extracted and try different combinations to obtain the complex relative permittivity. The square of the complex relative permittivity obtained using the extracted parameters are subtracted from the square of the complex relative permittivity obtained using experimental values. The squared differential term is then compared with a predetermined tolerance value which is near to zero and the iteration goes on until the preset value is reached. The variation in the modeling parameters is random; however, boundary limits have been set so that the extracted parameters meet the requirement of the FDTD method. Varying the modeling parameters in a random fashion is the most challenging part of the algorithm. If a linear method was used to vary the parameters, the computation time would have been much higher. Since the variation is random, it takes less time to find a combination of values that produces the least squared difference.

The boundary conditions that need to be maintained for the MDM parameters to be integrated in the FDTD algorithm are *Ïµ*
_{
âˆž
}â€‰>â€‰1, *Ïµ*
_{
s
}â€‰<â€‰*Ïµ*
_{
âˆž
} and *Ïƒ*â€‰â‰¥â€‰*Ïµ*
_{
o
}(*Ïµ*
_{
âˆž
}â€‰âˆ’â€‰*Ïµ*
_{
s
})/*Ï„*.

The flow chart of the optimization algorithm is given in FigureÂ 1. The algorithm has been developed solely for single-pole modeling parameter extraction. The accuracy of the obtained results reduces significantly if the modeling parameters for more complex curves are extracted using this optimization algorithm.

## Results and discussion

The extracted parameters for the five metals using our developed algorithm are presented in TableÂ 1. From the table it can be observed that a maximum RMS deviation of 1.62 occurs for Iridium which indicates the robustness and accuracy of our optimization algorithm.

The complex relative permittivity for each metal has been determined using both extracted parameters and experimental values. Then the real and imaginary parts have been separated from the complex relative permittivity and plotted which is presented in FigureÂ 2(i,v). The red color indicates the imaginary part while the blue color indicates the real part of the complex relative permittivity. The solid lines denote the extracted parameters and the dotted lines denote the experimental values. From the figure it is clearly visible that the real and imaginary parts of the complex relative permittivity obtained using extracted parameters agree very well with the real and imaginary parts of the complex relative permittivity obtained from the experimental values (Palik 1998).

The parameters obtained by Rakic *et al.*(Rakic et al. 1998) for Nickel exhibits an RMS deviation of 4.38 in the wavelength range of 0.6 to 1.1Â Î¼m and the parameters obtained by Pernice *et al.* (Pernice et al. 2007) for Nickel show an RMS deviation of as large as 24.11 whereas our obtained parameters show an RMS deviation of only 1.02. For Palladium, the RMS deviation for the parameters reported by Rakic *et al.*(Rakic et al. 1998) is 3.1251 while it is only 0.25 for our case within the wavelength range of 0.3 to 0.7Â Î¼m.

The optimization method we have developed adopts random variation of the modeling parameters which reduces the computation time significantly while maintaining an excellent degree of accuracy for the single-pole material models. This is evident from the RMS deviation comparison of our extracted parameters with the results reported by other researchers.

We have utilized single-pole Debye model to fit our curves for the materials while Rakic *et al*. (Rakic et al. 1998) have used a six-pole Lorentz-Drude model and Pernice *et al*. (Pernice et al. 2007) have used a four-pole model for the fitting purpose of the frequency dependent complex permittivity curve of metals. The more is the number of poles, the higher is the computation time required. Our single-pole model requires significantly less computation time in comparison to multiple-pole models. We have simulated both single-pole and six-pole models for Nickel in an intel Core v i5 processor based computer and found that the computation time is reduced by ~15% using our extracted parameters. The difference in the computation time would be even more noticeable for longer distances of propagation. Therefore, it is evident that our results are better than theirs in terms of both accuracy and computation time.

## Conclusion

We report the modified Debye model parameters for five metals obtained using a nonlinear optimization algorithm which are valid for a wide frequency range. The extracted parameters are expected to be useful for the integration of material properties in the simulation model and obtain more accurate results. The accuracy of the parameters has been verified by comparing them with the experimental values.

## References

Baba T, Watanabe R, Asano K, Koyama F, Iga K: Theoretical and experimental estimations of photon recycling effect in light emitting devices with a metal mirror.

*Japanese j of appl phys*1996, 35(1):97-100.Chang-Hasnain CJ, Harbison J, Hasnain G, Von Lehmen AC, Florez L, Stoffel N: Dynamic, polarization, and transverse mode characteristics of vertical cavity surface emitting lasers.

*Quant Electro, IEEE J*1991, 27(6):1402-1409. 10.1109/3.89957Hickernell RK, Sarid D: Long-range surface magnetoplasmons in thin nickel films.

*Optics letters*1987, 12(8):570-572. 10.1364/OL.12.000570Hunt N, Schubert E, Kopf R, Sivco D, Cho A, Zydzik G: Increased fiber communications bandwidth from a resonant cavity light emitting diode emitting at Î»â€‰=â€‰940 nm.

*Appl phys letters*1993, 63(19):2600-2602. 10.1063/1.110443Jin E, Xu X: Plasmonic effects in near-field optical transmission enhancement through a single bowtie-shaped aperture.

*Appl Phys B: Lasers and Optics*2006, 84(1):3-9.Katz A: Physical and chemical deposition of metals as ohmic contacts to InP and related materials. In

*Handbook of compound semiconductors*. Edited by: Holloway PH, McGuire GE. Park Ridge, NJ: Noyes Publications; 1995:170-250.Krug JT II, SÃ¡nchez EJ, Xie XS: Design of near-field optical probes with optimal field enhancement by finite difference time domain electromagnetic simulation.

*The J of chem phys*2002, 116: 10895. 10.1063/1.1479723Kunz KS, Luebbers RJ:

*The finite difference time domain method for electromagnetics*. Boca Raton, Florida USA: CRC Press; 1993.Luo H, Zory P: Distributed feedback coupling coefficient in diode lasers with metallized gratings.

*Photonics Techno Letters, IEEE*1990, 2(9):614-616.Ordal MA, Bell RJ, Alexander R Jr, Long L, Querry M: Optical properties of fourteen metals in the infrared and far infrared: Al, Co, Cu, Au, Fe, Pb, Mo, Ni, Pd, Pt, Ag, Ti, V, and W.

*Applied optics*1985, 24(24):4493-4499. 10.1364/AO.24.004493Palik ED:

*Handbook of optical constants of solids, vol 3*. San Diego, California, USA: Academic Press; 1998.Pernice WHP, Payne FP, Gallagher DFG: A general framework for the finite-difference time-domain simulation of real metals.

*Antennas and Propaga, IEEE Trans*2007, 55(3):916-923.Rakic AD, DjuriÅ¡ic AB, Elazar JM, Majewski ML: Optical properties of metallic films for vertical-cavity optoelectronic devices.

*Applied optics*1998, 37(22):5271-5283. 10.1364/AO.37.005271Shi X, Hesselink L: Design of a C aperture to achieve Î»/10 resolution and resonant transmission.

*JOSA B*2004, 21(7):1305-1317. 10.1364/JOSAB.21.001305Shi X, Thornton RL, Hesselink L: A nano-aperture with 1000Ã— power throughput enhancement for very small aperture laser system (VSAL). In

*Proceedings of the Optical Data Storage Conference (SPIE)*. Santa Fe, New Mexico, USA; 2002:320-327.Smith GM, Forbes DV, Lammert RM, Coleman JJ: Metallization to asymmetric cladding separate confinement heterostructure lasers.

*Appl phys letters*1995, 67(26):3847-3849. 10.1063/1.115293Yang L, Wu MC, Tai K, Tanbunâ€’Ek T, Logan RA: InGaAsP (1.3 Î¼m)/InP verticalâ€’cavity surfaceâ€’emitting laser grown by metalorganic vapor phase epitaxy.

*Appl phys letters*1990, 56(10):889-891. 10.1063/1.102619Yates C, Samuel I, Burn P, Wedge S, Barnes WL: Surface plasmon-polariton mediated emission from phosphorescent dendrimer light-emitting diodes.

*Appl phys letters*2006, 88(16):161103-161105. 10.1063/1.2195778Yee K: Numerical solution of initial boundary value problems involving Maxwellâ€™s equations in isotropic media.

*Antennas and Propaga, IEEE Trans*1966, 14(3):302-307.Zervas M: Surface plasmon-polariton fiber-optical polarizers using thin-nickel films.

*Photonics Techno Letters, IEEE*1990, 2(4):253-256.

## Acknowledgment

The authors would like to thank Ashik Ahmed, Assistant Professor, Department of Electrical and Electronic Engineering, Islamic University of Technology for helping in the revision process of the manuscript.

## Author information

### Authors and Affiliations

### Corresponding author

## Additional information

### Competing interests

The authors declare that they have no competing interests.

### Authorsâ€™ contributions

MGS designed and performed the experiment. MGS and RHS drafted the manuscript. MTAA and AAN prepared the figures and revised the manuscript. All authors read and approved the final manuscript.

## Authorsâ€™ original submitted files for images

Below are the links to the authorsâ€™ original submitted files for images.

## Rights and permissions

**Open Access**
This article is distributed under the terms of the Creative Commons Attribution 2.0 International License (
https://creativecommons.org/licenses/by/2.0
), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

## About this article

### Cite this article

Sagor, R.H., Saber, M.G., Al-Amin, M.T. *et al.* An optimization method for parameter extraction of metals using modified Debye model.
*SpringerPlus* **2**, 426 (2013). https://doi.org/10.1186/2193-1801-2-426

Received:

Accepted:

Published:

DOI: https://doi.org/10.1186/2193-1801-2-426

### Keywords

- Finite-difference time-domain
- Modified Debye model
- Metal optics
- Near-IR photonics